**HAL Id: hal-00957187**

**https://hal.archives-ouvertes.fr/hal-00957187**

### Submitted on 10 Mar 2014

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

**Specific heat measurements of a superconducting NbS2**

**single crystal in an external magnetic field: Energy gap**

**structure**

### J. Kačmarčík, Z. Pribulová, C. Marcenat, Thierry Klein, Pierre Rodière,

### Laurent Cario, P. Samuely

**To cite this version:**

### J. Kačmarčík, Z. Pribulová, C. Marcenat, Thierry Klein, Pierre Rodière, et al.. Specific heat

### measure-ments of a superconducting NbS2 single crystal in an external magnetic field: Energy gap structure.

### Physical Review B: Condensed Matter and Materials Physics (1998-2015), American Physical Society,

### 2010, 82, pp.014518. �10.1103/PhysRevB.82.014518�. �hal-00957187�

**Specific heat measurements of a superconducting NbS**

**2**

**single crystal in an external**

**magnetic field: Energy gap structure**

J. Kačmarčík,1_{Z. Pribulová,}1_{C. Marcenat,}1,2_{T. Klein,}3,4_{P. Rodière,}3_{L. Cario,}5 _{and P. Samuely}1

1_{Centre of Very Low Temperature Physics at Institute of Experimental Physics, Slovak Academy of Sciences,}

*Watsonova 47, SK-04001 Košice, Slovakia*

2* _{SPSMS, UMR-E 9001, LaTEQS, CEA-Institut Nanosciences et Cryogénie/UJF-Grenoble 1, 17 rue des martyrs, 38054 Grenoble, France}*
3

_{Institut Néel, CNRS, 38042 Grenoble, France}4* _{Institut Universitaire de France and Université Joseph Fourier, 38041 Grenoble, France}*
5

_{Institut des Matériaux Jean Rouxel, Université de Nantes–CNRS, 44322 Nantes, France}共Received 16 February 2010; revised manuscript received 19 May 2010; published 14 July 2010兲

The heat capacity of a 2H-NbS_{2}single crystal has been measured by a highly sensitive ac technique down
to 0.6 K and in magnetic fields up to 14 T. At very low temperatures, data show excitations over an energy gap
共2⌬*S*/*kBTc*⬇ 2.1兲 much smaller than the BCS value. The overall temperature dependence of the electronic

*specific heat Ce*can be explained either by the existence of a strongly anisotropic single-energy gap or within

a two-gap scenario with the large gap about twice bigger than the small one. The field dependence of the
Sommerfeld coefficient ␥ shows a strong curvature for both principal-field orientations, parallel*共H*储*c*兲 and
perpendicular* _{共H ⬜c兲 to the c axis of the crystal, resulting in a magnetic field dependence of the }*
supercon-ducting anisotropy. These features are discussed in comparison to the case of MgB2and to the data obtained by

scanning-tunneling spectroscopy. We conclude that the two-gap scenario better describes the gap structure of
NbS_{2}*than the anisotropic s-wave model.*

DOI:10.1103/PhysRevB.82.014518 PACS number共s兲: 74.25.Bt, 74.25.F⫺, 74.25.Ha, 74.70.Ad

**I. INTRODUCTION**

The old concept of multiband/multigap
super-conductivity1 _{has found its strong experimental evidence}

only recently in the rich physics of magnesium diboride.2

Consequently more superconductors are共re兲considered along
this line. One of the important examples are the iron
*pnic-tides, a new class of high-Tc* superconductors3 for which
multigap superconductivity is suggested to lead to an exotic
pairing mechanism with a sign reversal of the order
param-eter between separated Fermi-surface sheets. A revision in
dichalcogenides brings more and more signatures of a
distri-bution of superconducting energy gaps, which can be either
due to different gaps on different Fermi-surface sheets or
anisotropic single gap.

*Transition-metal dichalcogenides 2H-MX*2 *共M = Nb, Ta,*

*X*= S , Se兲 are materials with layered structure. Nb or Ta
at-oms are trigonally prismatic coordinated by chalcogen atat-oms
and metallic layers are held together by weak van der Waals
forces. Because of this layered structure, electrical, magnetic,
and optical properties show a high degree of anisotropy.
NbS2*is the only member of the 2H-MX*2family, which does

not undergo a charge-density wave transition.4_{This could be}

a reason for its strong anisotropy, much larger than that of NbSe2.

NbSe2 had been considered for a long time as being a

conventional type-II superconductor.5_{Later on, effects of the}

anisotropic and strong-coupling interactions were taken into
account.6,7 _{Recent measurements sensitive to the order }

pa-rameter show evidence that more than one energy scale is necessary to account for establishing superconductivity.8–12 NbS2 was also originally considered as just another

aniso-tropic superconductor and its unusual specific heat
depen-dence was not interpreted in detail.13,14_{An important }

break-through came with scanning-tunneling microscopy/

spectroscopy *共STM/STS兲 measurements by Guillamón et*

*al.*,15_{showing strong indications for two superconducting }

en-ergy gaps instead of a single anisotropic one. Since STM is a
surface probe, this strong statement certainly needs
indepen-dent support showing that the two gaps are reflecting the
bulk properties of the system. In this paper we address this
issue with bulk thermodynamic measurements of the specific
heat at temperatures down to 0.6 K and in magnetic fields up
to 14 T via ac-calorimetry technique. We find that the
*elec-tronic specific heat Ce*cannot be described by the standard
BCS model with a single isotropic energy gap. First, at the
lowest temperatures the data show that quasiparticles are
ex-cited over an energy gap much smaller than the BCS
*weak-coupling limit. The overall temperature dependence of Ce*
can be described only if two gaps or an anisotropic one gap
case is considered. Second, the field dependence of the
Som-merfeld coefficient ␥ shows a strong curvature in striking
similarity with that of NbSe2and MgB2. However, the

aniso-tropy of␥decreases with magnetic field in an opposite man-ner compared to the latter system. Finally, the two-gap sce-nario is supported by the absence of in-plane gap anisotropy in recent STM imaging of the vortex lattice in NbS2,15 and

by the fact that the numerical values of the two gaps obtained
from fitting our data, 2⌬*S*/*kBTc*⬇ 2.1 and 2⌬*L*/*kBTc*⬇ 4.6, are
also in a very good agreement with the STM data.

**II. EXPERIMENT**

Details of the synthesis of the single crystalline samples
can be found elsewhere.16 _{The crystals used for the specific}

heat measurements come from the same batch as those used
in the previous STM studies.15 _{Their chemical composition}

was checked using an energy dispersive x-ray spectroscopy. Single crystals were also confirmed to be of 2H polytype by x-ray diffraction measurements. In our experiment a thin

crystal with a well-defined hexagonal shape and dimensions
500⫻ 500⫻ 30 m3_{was chosen.}

Specific heat measurements have been performed using
an ac technique as described elsewhere.17The high
sensitiv-ity of this technique is not only very well adapted to measure
the specific heat of very small samples but also to carry
continuous measurements during temperature or magnetic
field sweeps. We were thus able to obtain the field
*depen-dence of the electronic part of C / T at T*⬇ 0.6 K which only
differs from its zero-temperature limit, the Sommerfeld
co-efficient ␥, by about 2%. Measurements were performed
with the magnetic field aligned along the two main
crystal-lographic orientations, i.e., parallel and perpendicular to the
*basal ab plane of the sample. The temperature oscillations of*
the sample were recorded by a thermocouple calibrated in
magnetic field using measurements on ultrapure silicon. We
performed measurements at temperatures down to 0.6 K and
in magnetic fields up to 8 T in the3He and4He refrigerators
in Košice. Supplementary measurements up to 14 T and
down to 2 K were performed in Grenoble.

**III. RESULTS AND DISCUSSION**

Figure1displays the temperature dependence of the
spe-cific heat of the sample共plus addenda兲 in selected magnetic
*fields up to 8 T for H*储*ab* *and up to 3 T for H*储*c*. The
ther-modynamic superconducting transition temperature at zero
field was determined from the local entropy balance around
*the phase transition giving Tc*= 6.05 K. The zero-field

anomaly at the transition is sharp *共⌬Tc*⬃ 0.4 K兲 indicating
the high quality and homogeneity of the sample. The position
of the specific heat jumps are gradually shifted toward lower
temperatures for increasing magnetic field. Despite a
signifi-cant broadening at high fields, the anomaly remains well
*resolved at all fields. A field of 3 T applied along the c axis*
was sufficient to completely suppress superconductivity in
all the temperature range. On the other hand, 8 T applied
*along the ab planes shifts the superconducting anomaly*
down to only about 3–4 K underlying the strong anisotropy
of this system.

Later we extended the measurements down to 0.6 K in a

3

He fridge where the specific heat was measured at zero field
*and at H*储*c*= 3 T. In the case of a very small crystal like
ours, it is difficult to evaluate the exact total contribution of
the addenda. The electronic part of the total specific heat
*value can be obtained by extrapolation of Ctot*/*T* for T
ap-proaching zero. This value corresponds to⬃38% of␥*n*, with
␥*nT* being the electronic heat capacity of the sample in the
normal state. To avoid any fitting procedures, the addenda
and the phononic contributions have been eliminated by
*sub-tracting the data taken at H*储*c*= 3 T from all the other runs.
*Thus, the electronic specific heat of the sample, Ce共T兲,*
normalized to its normal-state value, ␥*nT*, can be
obtained experimentally by: *Ce共T兲 /*␥*nT*=

⌬共C/T兲
␥*n* + 1,
where ⌬共C / T兲 = C共T , H = 0兲 / T − C共T , H = 3 T储*c兲 / T and* ␥*n*
= C共H = 3 T储*c兲 / T*兩0.6 K*− C共H = 0兲 / T*兩0.6 K. The result is

pre-sented in Fig.2 by the open circles. The only assumption in this procedure is the absence of magnetic field dependence of the addenda. This has been previously verified in numerous experiments using the same thermocouple wires and also

5
10
15
20
25
0, 0.2, 0.5, 0.8, 1, 1.3, 1.6,
2, 2.5, 3, 4, 5, 6, 7, 8 T
*a) H || ab*
*C*
/
*T*
(a
rb
.u
.)
2 3 4 5 6 7
5
10
15
20
25
*b) H || c*
0, 0.1, 0.2, 0.3, 0.4, 0.5,
0.7, 1, 1.2, 1.4, 1.6, 3 T
*C*
/
*T*
(a
rb
.u
.)
*T (K)*

*FIG. 1. Total specific heat C / T of NbS*_{2}in magnetic field 共a兲
parallel and*共b兲 perpendicular to the ab planes. In both data sets the*
zero-field measurement is the rightmost curve.

0.0 0.2 0.4 0.6 0.8 1.0
0.0
0.5
1.0
1.5
2.0
2.5
3.0
data
BCS
fit
*C*e
/
γn
*T*
*T / T*
c
1 2 3 4
0.1
1 *C*
e
/
γ
n* _{T}*
c

*T*c/

*T*

FIG. 2. Open circles: electronic specific heat of NbS2in zero

magnetic field extended down to 0.6 K. Dashed line: BCS
single-gap weak-coupling case. Solid line: two-gap model with
2⌬* _{S}*/

*k*= 2.1, 2⌬

_{B}T_{c}*/*

_{L}*k*= 4.6 and respective relative contributions ␥

_{B}T_{c}*S*/␥

*n*= 0.4, ␥

*L*/␥

*n*= 0.6. The anisotropic-gap model with anisotropy

parameter ␣ = 0.5 and 2⌬_{0}/*k _{B}T_{c}*= 3.6 follows essentially the same
line. Inset: exponential dependence of the specific heat, the full line
represents the best fit of the exponential decay, the dashed line is the
behavior expected for a BCS single-gap weak-coupling limit.

*KAČMARČÍK et al.* **PHYSICAL REVIEW B 82, 014518**共2010兲

confirmed here independently by the entropy conservation required for a second-order phase transition, proving the thermodynamic consistency of the data and its treatment.

We first compare the electronic specific heat with the iso-tropic single-gap共ISG兲 BCS model. The dashed line in Fig.2

presents the ISG-BCS specific heat 共weak coupling of
*2⌬ / kBTc*= 3.52兲. One can see that while the height of the
*jump at Tc*of the experimental data is quite well reproduced,
a significant deviation occurs at lower temperatures. The
dis-crepancy between the BCS curve and the measured data
rep-resents 18%共7%兲 of the total signal at 1.4 K 共4 K兲, which is
significantly larger than the error bars of our measurements.
The inset of Fig.2displays the logarithm of the electronic
*specific heat versus Tc*/*T*. As shown, one obtains an
*expo-nential dependence Ce*⬀ exp*共−b ⴱTc*/*T兲 for Tc*/*T*ⱖ 2.5.
*How-ever, the parameter b is significantly lower than the value*
expected for the BCS weak-coupling limit in the temperature
*range Tc*/*T*= 2.5– 4.5.18 This corresponds to coupling ratio
*2⌬ / kBTc*⬃ 2.3 that is much smaller than the ISG-BCS value
of 3.52, indicating that the quasiparticles are activated over a
small energy gap. This fact as well as the overall shape of the
specific heat temperature dependence resembles the case of
MgB2.

A phenomenological ␣ model of the specific heat ac-counting for independent contributions from two bands with two different energy gaps has been successfully applied in the case of MgB2.19 The magnitude of the small gap

2⌬*S*/*kBTc* and of the large gap 2⌬*L*/*kBTc* *at T = 0 are*
fitting parameters of the model. The third parameter is the
relative fraction of the density of states 共DOS兲 of the two
bands␥* _{S},n*/␥

*L,n*. The full line in Fig.2represents a fit to the

experimental data yielding the following parameters:
2⌬*S*/*kBTc*= 2.1⫾ 0.05, 2⌬*L*/*kBTc*= 4.6⫾ 0.2, and ␥*S,n*/␥*L,n*

= 0.67⫾ 0.15. The value of the small gap is close to the one evaluated from the exponential decay shown in the inset of Fig.2. Importantly, both gap values are in striking agreement with those found in the STM experiment15 confirming that the latter are characteristic of the bulk.

*As previously shown by Huang et al.,*10 _{the temperature}

dependence of the specific heat of NbSe2, another two-gap

superconductor, can also be described by an anisotropic

*s*-wave model, where the gap anisotropy is supposed to be in
the form of ⌬ = ⌬0共1 +␣cos 6兲 corresponding to the

hex-agonal in-plane symmetry. Here, ⌬0is the average gap value

and ␣ denotes its anisotropy, yielding ⌬*max*= ⌬0共1 +␣兲 and

⌬*min*= ⌬0共1 −␣兲. This model with parameters ␣= 0.5 and

2⌬0/*kBTc*= 3.6 fits our data as well as the two-gap scenario,

*the difference between the two models is negligible*. We
re-mark that the anisotropic gap should leave its footprint in the
anisotropic vortex core as it is proportional to the related
*Fermi velocity vF* divided by the gap at zero temperature
⌬共0兲. However, in contrast to NbSe2, for which STS images

revealed a sixfold star shape of the vortex cores, the fully isotropic vortices have been imaged in NbS2 共Ref.15兲

ques-tioning the applicability of the anisotropic single-gap model in our case.

We have measured thoroughly the evolution of the
*cific heat in the mixed state. At T = 0.6 K the electronic *
*spe-cific heat term Ce*/*T* is very close to the Sommerfeld
coeffi-cient ␥. Its field dependence is displayed in Figs. 3共a兲 and

3共b兲for both principal field orientations. Our maximum field
available at this temperature range共8 T兲 was not sufficient to
*reach the normal state for H*储*ab*, but it was well above the
*upper critical-field value of 2.4⫾ 0.1 T for H*储*c*. Figure3共a兲

emphasizes the strong nonlinearity of ␥*共H兲 when H is *
*ap-plied perpendicular to the ab plane. Again, such a *
nonlinear-ity could be associated with the existence of two gaps or a
single anisotropic one.

The increase in␥with magnetic field is mainly due to the
quasiparticle contribution inside the vortex cores. In the case
of superconductor with a single isotropic gap, ␥ should
in-crease linearly in small magnetic field and a small
nonlinear-ity in ␥*共H兲 appears above the field where flux lines start*
*overlapping. According to the calculations of Nakai et al.,*20

much stronger nonlinearity of ␥*共H兲 is achieved in case of*
anisotropic-gap superconductors. The full line in Fig. 3共a兲

displays the field dependence of the normalized density of
*states N共B兲 / N*0 共proportional to the Sommerfeld coefficient兲

*calculated by Nakai et al. for the anisotropic gap with* ␣
1
2
0.0 0.1 0.2
0 1 2 3 4 5 6 7 8
0.0
0.2
0.4
0.6
0.8
1.0
0 2 4 6 8 10 12 14 16
0.0
0.2
0.4
0.6
0.8
1.0
0.0 0.2 0.4 0.6 0.8 1.0
0.0
0.2
0.4
0.6
0.8
1.0 _{NbS}
2
*H|| c*
*T*= 0.6 K
a)
γ
(
*H*
)/
γN
*H _{/H}*
c2
c

*H/H*c2 c δ [ γ (

*H*)/ γN ]/ δ

*[H*

*/H*c2 c ] NbS

_{2}

*T*= 0.6 K

*H||ab*b)

*H|| c*

*H*

_{(T)}γ (

*H*)/ γN MgB 2

*T*= 2.5 K

*H||ab*

*H|| c*c) γ (

*H*)/ γN

*H*

_{(T)}

FIG. 3. 共a兲 Open circles: normalized Sommerfeld coefficient ␥
*as a function of magnetic field perpendicular to the ab planes of*
NbS_{2}. Line: model accounting for highly anisotropic gap with ␣
= 0.5共Ref.20兲. Inset is the derivative of the corresponding curves
from the main panel: open circles–of the measured data, line–of the
model.共b兲 and 共c兲 ␥ / ␥*n*for both orientations of the magnetic field

= 0.5. The model qualitatively reproduces the behavior in our
data 共open circles兲, but fails to describe the fast increase in
␥*共H兲 at low fields. This is evident in the inset of Fig.*3共a兲

where the derivative * _{N}_{共B兲 /}*

*␣= 0.5共line兲 and the slope of measured Sommerfeld coeffi-cient ␥*

_{B}_{, i.e., the slope of N共B兲 for}*共H兲 /*

*H*共open circles兲 are compared. This discrep-ancy makes the explanation of the specific heat data by the anisotropic-gap scenario rather inconsistent. The observed ␥

*共H兲 behavior resembles the two-gap case of MgB*2关see Fig.

3共c兲, left curve兴,21 _{where the initial rapid increase in} _{␥}_{共H兲}

due to dominant role of the band with the small gap changes at fields where theband with the large gap comes into play.

Next, we compare the behavior of the Sommerfeld coef-ficients in magnetic fields applied parallel and perpendicular to the basal planes of the both materials, NbS2 关Fig. 3共b兲兴

and MgB2关Fig.3共c兲兴. The latter is taken from Ref.21.

*Fol-lowing the procedure introduced by Bouquet et al. in Ref.*22

an effective anisotropy ⌫*ef f*can be obtained from these␥*共H兲*
dependences. It is defined as the ratio of the magnetic fields
*in the ab plane and along the c axis yielding the same* ␥
value in Figs. 3共b兲 and3共c兲. ⌫*ef f* is plotted in Fig. 4共a兲for
*both compounds as a function of the field H*储*c*normalized to
*its upper critical-field value Hc*2 储*c*. As discussed already in

*the work of Bouquet et al.*22 _{on MgB}

2 the choice of the

*abscissa is arbitrary. We chose H*储*c*, but we could plot ⌫*ef f*
*versus H*储*ab*or versus␥*共H兲 as well. Note that this ⌫ef f*tends
*toward the usual anisotropy of Hc*2, ⌫ =

*Hcab*2

*Hcc*2 when

␥
␥*n*→ 1 at
large magnetic fields. In MgB2 at low fields共

*H*

*Hcc*2⬍ 0.1兲, the

␥*共H兲 curves for the two principal directions are practically*
identical which gives ⌫*ef f*= 1 as shown in Fig.4共a兲. At larger
fields, ⌫*ef f* increases reflecting a reduced contribution from

the isotropic band, reaching ⌫*ef f*⬃ 5, which is the
aniso-tropy of the dominant band.21 _{In NbS}

2, one observes an

opposite field dependence of ⌫*ef f*which starts from a highly
anisotropic value ⌫*ef f*⬃ 10 at low fields and decreases to
⌫*ef f*⬃ 5.5 at our maximum field. A field-dependent
supercon-ducting anisotropy is a typical signature of multigap
super-conductivity where a role of bands with different gaps can
significantly vary with magnetic field.23–25 _{In contrast to}

MgB2 case, in NbS2 both bands would be anisotropic, as

suggested by analogy with NbSe2 in which band-structure

calculations26_{show mostly four Fermi-surface sheets derived}

*from Nb d bands forming warped cylinders along the c axis,*
centered on the ⌫ and K points in the Brillouin zone.
*More-over, two sheets derived from the bonding Nb d band are*
significantly more warped than the two derived from the
*an-tibonding Nb d band. Different warping of Nb sheets can*
naturally lead to a different level of anisotropy in each band.
Thus, a qualitatively different behavior of ⌫*ef f共H兲 compared*
to MgB2can be expected.

Finally, we inspected the upper critical magnetic fields for
both principal orientations of magnetic field. Figure 5
*sum-marizes the values of Hc*2 derived from the

temperature-sweep measurements of the specific heat shown in Fig.1, as
well as from field-sweep measurements. Two sets of field
*sweeps were performed, one in 14 T magnet for H*储*ab* in a
temperature range down to 2 K, and another one taken in the

3

He cryostat down to 0.6 K in the 8 T coil. As stated above,
*we determined Tc*at zero field from the local entropy balance
around the anomaly. However, at finite fields this definition
*is not very practical for establishing Tc*2*共H兲, or Hc*2*共T兲. In*

*order to reduce the uncertainty of the Hc*2value arising from

the broadening of the transition particularly at lower
tem-peratures 共higher fields兲, we inspected the temperature shift
between two neighboring curves in Fig. 1. A similar
*proce-dure was used to determine Hc*2 from field-sweep

*measure-ments. The resulting temperature dependence of Hc*2 is

shown in Fig. 5*for both H*储*ab* *and H*储*c*.

0.0 0.2 0.4 0.6 0.8 1.0
0
2
4
6
8
10
12
0.0 0.2 0.4 0.6 0.8 1.0
2
3
4
5
6
7
8
MgB_{2}
NbS_{2}
b)
Γ
*(T*
)
*T/T*c
a)
MgB
2
NbS
2
Γe
ff
*(H*
)
*H/H*c2
c

FIG. 4. Anisotropy of NbS_{2} 共full circles兲 compared to MgB2

共Refs.21and 27兲 共open circles兲: 共a兲 field dependence of effective anisotropy defined as the ratio of the fields applied in both principal orientations that correspond to the same ␥ value in Figs.3共b兲and

3共c兲*共b兲 temperature dependence of anisotropy ⌫ = H _{c}ab*

_{2}

_{/}

_{H}*c*2

*c*

_{.}0 1 2 3 4 5 6 0 4 8 12 16

*H*

_{|| c}*H*

_{|| ab}*H*c2 (

*T*)

*T*

_{(K)}

*FIG. 5. Upper critical field Hc*2 for magnetic field 储*ab* 共full

circles result from temperature-sweep measurements, full triangles
from field sweeps兲 and 储*c* 共open circles result from
temperature-sweep measurements, open triangles from field temperature-sweeps兲.

*KAČMARČÍK et al.* **PHYSICAL REVIEW B 82, 014518**共2010兲

Importantly, the three independent sets of temperature and
field-sweeps measurements yield consistent results with a
nice overlap. Both temperature dependencies show a slight
*positive curvature for temperatures T ⬎ Tc*/2. The upper
*criti-cal field in the ab plane reveals very high values with*

*dHc*2/*dT*slope of about 3 T/K, close to the Pauli

paramag-netic limit.

The temperature dependence of the superconducting
*an-isotropy ⌫ calculated as a ratio Hc*2 储*ab / Hc*2 储*c* of the upper

critical fields is displayed in Fig. 4共b兲 together with the re-sults obtained in MgB2.27As shown, in contrast to MgB2, the

resulting anisotropy ⌫ is close to 7 and approximately
*con-stant for T / Tc*⬎ 0.3. Note that this value might be slightly
underestimated in case of a small misalignment of the crystal
*for H*储*ab*. Our results are consistent with those obtained by
*Onabe et al.*28_{from resistive measurements in a field up to 2}

T. The strong decrease in ⌫ in MgB2*close to Tc*is a direct
consequence of the existence of the isotropicband. This is
not a general feature of multiband superconductivity since
⌫共T兲 results from a subtle balance between the Fermi
veloci-ties and the relative weight in the DOS of the different
bands.24_{These precise calculations are still to be carried out}

in the case of NbS2.

**IV. CONCLUSIONS**

Analysis of the zero-field specific heat data has shown that: 共1兲 the zero-field electronic term of the specific heat

cannot be described by an isotropic single-gap BCS formula
but it is compatible with the two-gap ␣model;共2兲 the large
共small兲 gap is 2⌬*L*/*kBTc*⬇ 4.6 共2⌬*S*/*kBTc*⬇ 2.1兲. The
mea-surements in the mixed state have supported the two-gap
scenario revealing:共3兲 a strongly nonlinear␥*共H兲; 共4兲 a *
field-dependent superconducting anisotropy. Even if some of these
features of the specific heat could be eventually explained by
an extremely anisotropic-gap superconducting model, this
would not be compatible with the observation of two
well-resolved gap features with sizes of 2⌬*S*/*kBTc*⬇ 2 and 4,
re-spectively, and also with the absence of in-plane anisotropy
in the vortex lattice images by the scanning-tunneling
*spec-troscopy of Guillamón et al. To conclude, our bulk *
thermo-dynamic measurements are in full agreement with STM
spectra, supporting that NbS2 is another case of

well-resolved two-gap superconductor.

**ACKNOWLEDGMENTS**

This work was supported by the EC Framework Pro-gramme under Grant No. MTKD-CT-2005-030002, by the EU ERDF 共European regional development fund兲 under Grant No. ITMS26220120005, by the Slovak Research and Development Agency, under Grants No. VVCE-0058-07, No. APVV-0346-07, No. SK-FR-0024-09, and No. LPP-0101-06, and by the U.S. Steel Košice, s.r.o. Centre of Low Temperature Physics is operated as the Centre of Excellence of the Slovak Academy of Sciences. We thank G. Karapetrov for careful reading of the manuscript.

1_{H. Suhl, B. T. Matthias, and L. R. Walker,} _{Phys. Rev. Lett. 3,}

552共1959兲.

2_{X. X. Xi,}_{Rep. Prog. Phys. 71, 116501}_{共2008兲.}

3_{Superconductivity in Iron-Pnictides}_{, edited by P. C. W. Chu,}

A. Koshelev, W. Kwok, I. Mazin, U. Welp, and H.-H. Wen,
special issue of**Physica C 469**共9-12兲, 313 共2009兲.

4_{D. E. Moncton, J. D. Axe, and F. J. DiSalvo,}_{Phys. Rev. Lett. 34,}

734共1975兲.

5_{B. T. Matthias, T. H. Geballe, and V. B. Compton,} _{Rev. Mod.}

**Phys. 35, 1**共1963兲.

6_{N. Kobayashi, K. Noto, and Y. Muto,} _{J. Low Temp. Phys. 27,}

217共1977兲.

7_{D. Sanchez, A. Junod, J. Muller, H. Berger, and F. Lèvy,}_{Physica}

**B 204, 167**共1995兲.

8_{T. Yokoya, T. Kiss, A. Chainani, S. Shin, M. Nohara, and}

H. Takagi,**Science 294, 2518**共2001兲.

9_{J. D. Fletcher, A. Carrington, P. Diener, P. Rodière, J. P. Brison,}

R. Prozorov, T. Olheiser, and R. W. Giannetta,Phys. Rev. Lett.

**98, 057003**共2007兲.

10_{C. L. Huang, J.-Y. Lin, Y. T. Chang, C. P. Sun, H. Y. Shen, C. C.}

Chou, H. Berger, T. K. Lee, and H. D. Yang,**Phys. Rev. B 76,**
212504共2007兲.

11_{T. Kiss, T. Yokoya, A. Chainani, S. Shin, T. Hanaguri, M. }

No-hara, and H. Takagi,**Nat. Phys. 3, 720**共2007兲.

12_{T. Valla, A. V. Fedorov, P. D. Johnson, P.-A. Glans, C. }

McGuin-ness, K. E. Smith, E. Y. Andrei, and H. Berger,Phys. Rev. Lett.

**92, 086401**共2004兲.

13_{Y. Hamaue and R. Aoki,}_{J. Phys. Soc. Jpn. 55, 1327}_{共1986兲.}
14_{D. C. Dahn, J. F. Carolan, and R. R. Haering,}_{Phys. Rev. B 33,}

5214共1986兲.

15_{I. Guillamón, H. Suderow, S. Vieira, L. Cario, P. Diener, and}

P. Rodière,**Phys. Rev. Lett. 101, 166407**共2008兲.

16_{W. Fisher and M. Sienko,}_{Inorg. Chem. 19, 39}_{共1980兲.}
17_{P. F. Sullivan and G. Seidel,}_{Phys. Rev. 173, 679}_{共1968兲.}
18_{Superconductivity}_{, edited by R. D. Parks}_{共Marcel Dekker, New}

York, 1969兲.

19_{F. Bouquet, Y. Wang, R. A. Fisher, D. G. Hinks, J. D. Jorgensen,}

A. Junod, and N. E. Phillips,**Europhys. Lett. 56, 856**共2001兲.

20_{N. Nakai, P. Miranović, M. Ichioka, and K. Machida,}_{Phys. Rev.}

**B 70, 100503共R兲 共2004兲.**

21_{Z. Pribulová, T. Klein, J. Marcus, C. Marcenat, F. Levy, M. S.}

Park, H. G. Lee, B. W. Kang, S. I. Lee, S. Tajima, and S. Lee,

**Phys. Rev. Lett. 98, 137001**共2007兲.

22_{F. Bouquet, Y. Wang, I. Sheikin, T. Plackowski, A. Junod,}

S. Lee, and S. Tajima,**Phys. Rev. Lett. 89, 257001**共2002兲.

23_{V. G. Kogan and S. I. Bud’ko,}_{Physica C 385, 131}_{共2003兲.}
24_{T. Dahm and N. Schopohl,}_{Phys. Rev. Lett. 91, 017001}_{共2003兲.}
25_{A. A. Golubov, A. Brinkman, O. V. Dolgov, J. Kortus, and}

O. Jepsen,**Phys. Rev. B 66, 054524**共2002兲.

26_{M. D. Johannes, I. I. Mazin, and C. A. Howells,}_{Phys. Rev. B}

**73, 205102**共2006兲.

27_{L. Lyard, P. Samuely, P. Szabo, T. Klein, C. Marcenat, L. }

Pau-lius, K. H. P. Kim, C. U. Jung, H.-S. Lee,B. Kang, S. Choi, S.-I.
Lee, J. Marcus, S. Blanchard, A. G. M. Jansen, U. Welp,
G. Karapetrov, and W. K. Kwok, **Phys. Rev. B 66, 180502共R兲**
共2002兲.

28_{K. Onabe, M. Naito, and S. Tanaka,} _{J. Phys. Soc. Jpn. 45, 50}